Tensile Strength of Natural Fibres Composite
Noor Azlina Abdul Hamid1*, Nur Azureen Fazilah Othman1, Norhafizah Salleh1
1Jamilus Research Center, Faculty of Civil and Environmental Engineering, Universiti Tun Hussein Onn Malaysia, 86400, Batu Pahat, Malaysia firstname.lastname@example.org
Natural fibres are the most potential material to be used as alternative fibres to replace the synthetic fibres used in composite materials as it abundantly available in our country. An experimental work was carried out in order to determine the tensile strength of natural fibres composite plates made of banana, sugarcane, and bamboo. The influence of combination among natural fibres which are composites plates of banana-sugarcane and banana-bamboo on tensile strength were investigated. The effect of fibres orientation with different angles of 00 and 450 on tensile strength was also investigated. The natural fibres were fabricated as composite plates with size of 25 mm x 230 mm and thickness less than 3 mm. From tensile test, it was found that the natural fibres composite plates with angle of 00 produces higher tensile strength compared to natural fibres composite plates with angle of 45˚. Moreover, the combination of natural fibres of banana-sugarcane and banana-bamboo produces higher tensile strength rather than composite plates of banana, sugarcane and bamboo itself.
Keywords— natural fibres, tensile strength, composite plate, bamboo, banana, sugarcane
Polymer composite is a combination of synthetic fibres such as glass (GFRP), carbon (CFRP) or aramid (AFRP) with matrix polymer such as polyester, vinyl-ester or epoxy. The use of synthetic fibres reinforced polymer composites has main advantage of high tensile strength compared to conventional reinforcement materials of steel [1,2]. These materials are being used in aerospace, automobile and civil engineering as structural materials which are relatively expensive.
The studies of fibres with low cost and high performance are required to produce economical and sustainable materials. Mankind has been used plant fibres for many kinds of purposes. Natural fibres such as banana, sugarcane and bamboo which are abundantly available in our country are potentially to be used as alternative fibres. These natural fibres are able to give certain benefits to the composites such as low density, low cost, recyclability, biodegradability and flexibility during processing. The advantages of natural fibres are utilized to reduce the use of synthetic fibres which are generally non-environmentally friendly. The utilization of natural resources and wastes are strongly encouraged due to the economical materials and awareness on the environmental impact and sustainability.
However, there is not much available information regarding to the natural fibres especially on their tensile strength and potential as alternative reinforcing materials. Hence, this research focuses on determining the tensile strength of natural fibres with different combination and orientation of natural fibres.
2. NATURAL FIBRES
A natural fibre is hair-like materials that are continuous filament. Traditionally, natural fibres are used for rope and twine materials and they are biodegradable and environmentally friendly crop. Natural fibres play an important role in developing recyclability composites to resolve the current environmental problems. Natural fibres are light, renewable, high strength and inexpensive resources.
The variations of natural fibres properties are influenced by the way plant are harvested and processed. They can be used as a component of composite materials. The development of natural fibres reinforced composites to replace synthetic fibres like glass and carbon as engineering applications has been performed due to the combination of interesting mechanical and physical properties together with their sustainable character . Table 1.1 shows the comparison of mechanical properties between the natural fibres of banana, sugarcane and bamboo.
Table 1.1: Mechanical properties of natural fibre (alkbir et al., 2016) Fibres Tensile strength
(MPa) Young’s modulus (GPa) Banana 53.7 3.48 Sugarcane 169.51 5.18 Bamboo 215-218 28-30 2.1 Banana Fibre
Banana fibre is a waste product of banana cultivation and easily available in tropical countries like Malaysia. Banana is one of the earliest and important fruit crop cultivated in tropical parts of the world . Banana farming generates huge quantity of biomass all of which goes as waste and the major source of fibre is the above ground parts like pseudostem and peduncle. Fig. 1.1 shows the part of banana which is pseudostem. Banana farming generated huge quantities of biomass all of which goes as waste due to non-availability of suitable technology for its commercial utilization. Normally this biomass is used for animal feed and most of it goes as wastes.
Figure 1.1: The pseudostem of banana
However, banana fibre is the best source of fibre that can be used in industry for production of paper, cardboards and reinforced as polymer composite with high quality materials. The physical properties of the banana fibres are shown in Table 1.2.
Table 1.2: Physical properties of banana fibre (Ramesh et al., 2014)
Property Range value
Cellulose (%) 63-64 Hemi cellulose (%) 19 Lignin (%) 5 Moisture (%) 10-11 Density (g/cm3) 1-1.5 Elongation at break (%) 4.5-6.5 Microfibrillar angle (deg.) 11
2.2 Sugarcane Fibre
It was indicated that sugarcane is a very tall grass with big stems . The main residues and by products of sugarcanes are bagasse and straw, defined here as the leaves of the sugarcane. Fig. 1.2 shows the fibrous residue of sugarcane after crushing and extraction of its juice, known as ‘bagasse’.
Fig. 1.2: Bagasse (sugarcane) wastes
Bagasse fibres have biodegradable and disposable properties and make it one of the most beneficial natural fibres. Table 1.3 shows the physical properties of bagasse fibre but the residue of sugarcane creates air pollution when it is burnt off. The bagasse fibre has many advantages due to its lower ash content compared to other residual crops such as rice straw and wheat straw. Sugarcane bagasse fibres are suitable for paper making and extensively used for making furniture, fiberboard and insulating board. Sugarcane rind fibres are also successfully used in textile and geotextile applications .
Table 1.3: Physical properties of bagasse fibre (Hossain et al., 2014) Property Percentage (%) Cellulose 35 Hemicellulose 36 Lignin 16 Water content 4 2.3 Bamboo Fibre
Bamboo is belongs to more than 10 genera including about 1450 species ranging from small annuals to giant timber bamboo and it is one of the
oldest building materials used by mankind . It is the fastest growing
woody plant in the world and is easily obtained globally. Fig. 1.3 shows the part of bamboo which is stems.
It was stated that a diverse range of products from domestic to industrial applications has been made from the bamboo culm or stem . The examples of bamboo products are food containers, skewers, chopsticks, handicrafts, toys, furniture, flooring, paper, boats, charcoal, musical instruments, weapons, bicycles, dirigibles, windmills, scales, retaining walls, ropes and cables.
Table 1.4 shows chemical composition of bamboo. Technologies have been extensively developed in recent years to process bamboo and make it more durable and usable as a building material with advances in science and technology and the restricted supply of timber.
Table 1.4: Chemical composition of bamboo (Nahar & Hassan, 2012)
Property Range (%)
Bamboo has also gained popularity as a ‘green’ fibre as it can be cultivated quickly and is a natural fibre which cultivation actually reduces greenhouse gases. A chemical process, mechanical needling and scraping or a steam explosion process can be used to extract the fibres from the leaves, branches and trunks. Bamboo is extremely resilient and durable as a fibre and has served as a foundation structure . For the past several years, bamboo fibre has been considered as an important plant fibre and has good potential to be used as reinforcement in polymer composites. Its characteristics, mechanical properties and thermal properties had made it a useful material for applying in engineering application.
3. FABRICATION OF NATURAL FIBRES COMPOSITE PLATES
The natural fibres used in this study are banana, sugarcane and bamboo. The fibres were separated and extracted from the stem of the plants manually. The fibres were sun-dried for a week and the manual process of shredded natural fibres was carried out. Fig. 1.4 shows the shredded fibres of banana.
Fig. 1.4: Shredded fibres of banana
The suitable method used for make the unidirectional natural fibres layer is by hand lay method. The fibres were combed carefully to form unidirectional oriented fibres. Then, epoxy resin was applied on them by using a small brush and had been dried for 24 hours at room temperature. Each layer of the fibres had thickness approximately 0.5 mm, 125 mm width and 250 mm length. The layer of the fibres was put on the aluminum plate. Additional layers were stacked up by following the procedure described above until required thickness of fibres composite plates is reached. The designation of natural fibres composite plates can be shown in Table 1.5. There are five types of natural fibres composite plates with different types of fibres and orientation of fibres. To provide better gripping and to avoid slipping of the composites plate during mechanical testing, the end tab of 50 mm were prepared. Fig. 1.5 shows the geometry of the sample of natural fibres composite plates.
Table 1.5: Natural fibre composites plates
Designation Type of natural fibre composites plate
No. of samples (orientation
angle) 0˚ 45˚
A Banana fibre reinforce
polymer 3 3
B Sugarcane fibre reinforce
polymer 3 3
C Bamboo fibre reinforce
polymer 3 3
AB Banana-sugarcane fibre
reinforce polymer 3 3
AC Banana-bamboo fibre
reinforce polymer 3 3
Fig. 1.5: Geometry of composite plate model
The Universal Testing Machine (UTM ) was used in order to determine the tensile strength of the composite plates of fibres. Accordingly, ASTM D3039 was being used as references in conducting the tensile test.
4. TENSILE STRENGTH OF NATURAL FIBRES
From the test results, it can be seen that the rupture of the composite plates does not occurred at the middle length of the sample but within the gage length as shown in Fig. 1.6. However, the result is still acceptable because the stress value is similar in the entire gage length. A cracking sound can be heard prior failure which indicates the rupture of the fibres.
Fig. 1.6: Sample of banana fibres composite plates with orientation (a) 00(b) 450 The tensile strength of the sample is calculated by dividing the maximum load with the area of the composite plate (width, b x thickness, d). From the tensile test results, different types and orientation angles of the natural fibres resulted variation on the tensile strength. Accordingly, the tensile strength of natural fibres for sample A (banana), sample B (sugarcane), sample C (bamboo), sample AB (banana-sugarcane) and sample AC (banana-bamboo) with different orientation angle of 0˚ and 45˚ of the fibres composite are plotted in Fig. 1.7 and 1.8.
From the figure, it is shows that the natural fibres composite plates with orientation angle of 0˚ had higher tensile strength than orientation angle of 45˚. The reason can be due to longer length of fibres with angle of 0˚ lead to higher tensile strength compared to short fibres due to orientation angle of 45˚. Hence, the lower angle of fibres, the higher tensile strength of natural fibres was obtained.
As shown in Fig. 1.7, the highest tensile strength was occurred in sample C which consist of bamboo fibres about 50.90 MPa. Thus, it indicated that the bamboo gave higher strength than other fibres such as banana and sugarcane. However, the combination of different natural fibers between banana and sugarcane in sample AB and between banana and bamboo in sample AC not significantly increased the tensile strength of the fibers.
Fig. 1.7: Tensile strength of natural fibre composites with 00angle 0 10 20 30 40 50 60 A B C AB AC Types of sample T e n s ile s tre n g th ( M Pa )
0.047 0.048 0.049 0.05 0.051 0.052 0.053 0.054 A B C AB AC
Fig. 1.8: Tensile strength of natural fibre composites with 450angle
From this study, the effect of orientation angle on tensile strength of fibres can be seen. It is indicated that the 0˚ angle of natural fibres gave higher tensile strength compared to natural fibres with angle of 45˚. The reason can be due to longer length of fibres with angle of 0˚ that lead to higher strength, stiffness and toughness compared to the natural fibres with short length due to angle of 45˚. Besides that, it was found that the combination of natural fibres between banana and sugarcane not significantly affect the tensile strength of composite plate. While, the combination of banana and bamboo was slightly increased the tensile strength of composite plate. It can be due to contribution of bamboo which has higher tensile strength compared to other types of natural fibres. This combination of fibres has provided considerable improvement on tensile strength.
It can be concluded that the potential types of natural fibres which can substitute synthetic fibres is bamboo as it shows higher tensile strength. The bamboo fibres are able to give certain benefits to the composites such as low density, low cost, recyclability, biodegradability and flexibility during process. Due to low density of the natural fibers used compared to the
T e n s ile s tre n g th ( M Pa ) Types of sample
synthetic fibres the composites can be regarded as a useful lightweight material.
The authors would like to thank the Faculty of Civil and Environmental Engineering, UTHM and Universiti Teknologi Malaysia, UTM for the given supports towards this study.
 N.A.A. Hamid, R. Thamrin, A. Ibrahim and H.A. Hamid, “Strain distribution on reinforcement of concrete beams reinforced with glass fiber reinforced polymer (GFRP) bars”, Key Engineering Materials, vol. 594-595, pp. 812-817, 2014
 N.A.A. Hamid, A. Ibrahim, R. Thamrin, and H.A. Hamid, “Experimental investigation on the shear behaviour of concrete beams reinforced with GFRP reinforcement bars”, Advanced Materials Research, vol. 626, pp. 559-563, 2013
 B. Ren, T. Mizue, K. Goda and J. Noda, “Effects of fluctuation of fibre orientation on tensile properties of flax sliver-reinforced green composites”, Journal Composite Structures, vol. 94, pp. 3457-3464, 2012
 P. Preethi and M.G. Balakrishna, “Physical and chemical properties of banana fibre extracted from commercial banana cultivars grown in Tamilnandu State, Agrotechnology, S11, 2013
 M.K. Hossain, M.R. Karim, M.R. Chowdhury, M.A. Imam, M. Hosur, S. Jeelani and R. Farag, “Comparative mechanical and thermal study of chemically treated and untreated single sugarcane fiber bundle”, Journal Industrial Crops and Products, vol. 58, pp. 78-90, 2014
 M. Kamruzzaman, S. Saha, A. Bose and M. Islam, “Effects of age and height on physical and mechanical properties of bamboo”, Journal Topical Forest Science, vol. 20, pp. 211-217, 2008.
 H.P.S.A. Khalil, M.S. Alwani, M.N. Islam, S.S. Suhaily, R. Dungani, Y.M.H. Ng and M. Jawaid, “The use of bamboo fibres as reinforcements in composites”, Biofiber Reinforcements in Composite Materials, Chapter: 16, pp. 488-524, 2015
 P.N. Khanam, H.A. Khalil, G.R. Reddy and S.V. Naidu, “Tensile, flexural and chemical resistance properties of sisal fibre reinforced polymer composites: Effect of fibre surface treatment”, Journal of Polymers and the Environment, vol. 19(1), pp. 115-119, 2011